markdown:
5 trang
Lượt xem: 156
Download: 80
# TC ASTM C42/C42M
Chia sẻ:
[daisyshop](http://tailieu.vn/user/daisyshop)
Phương pháp thử tiêu chuẩn về lấy mẫu và thử nghiệm lõi khoan và đà xẻ của bê-tông
## Thể loại:
[Kinh Tế - Quản Lý](http://tailieu.vn/kinh-te-quan-ly/)» [Tiêu chuẩn - Qui Chuẩn](http://tailieu.vn/kinh-te-quan-ly/tieu-chuan-qui-chuan/)
## Chủ đề liên quan:
**Nội dung Text: TC ASTM C42/C42M**
Designation: C 42/C 42M – 03 Highway and Transportation Officials Standard
AASHTO No.: T24
Standard Test Method for
Obtaining and Testing Drilled Cores and Sawed Beams of
Concrete1
This standard is issued under the ﬁxed designation C 42/C 42M; the number immediately following the designation indicates the year
of original adoption or, in the case of revision, the year of last revision. A number in parentheses indicates the year of last reapproval.
A superscript epsilon (e) indicates an editorial change since the last revision or reapproval.
This standard has been approved for use by agencies of the Department of Defense.
1. Scope C 642 Test Method for Density, Absorption, and Voids in
1.1 This test method covers obtaining, preparing, and test- Hardened Concrete2
ing (1) cores drilled from concrete for length or compressive C 670 Practice for Preparing Precision and Bias Statements
strength or splitting tensile strength determinations and ( 2) for Test Methods for Construction Materials2
beams sawed from concrete for ﬂexural strength determina- C 823 Practice for Examination and Sampling of Hardened
tions. Concrete in Constructions2
1.2 The values stated in either inch-pound units or SI units C 1231/C 1231M Practice for Use of Unbonded Caps in
shall be regarded separately as standard. SI units are shown in Determination of Compressive Strength of Hardened Con-
brackets. The values stated in each system may not be exact crete Cylinders2
equivalents; therefore, each system must be used indepen- 2.2 ACI Standards:
dently of the other. Combining values from the two systems 318 Building Code Requirements for Structural Concrete3
may result in non-conformance with the standard. 3. Signiﬁcance and Use
1.3 The text of this standard references notes and footnotes
that provide explanatory material. These notes and footnotes 3.1 This test method provides standardized procedures for
(excluding those in tables and ﬁgures) shall not be considered obtaining and testing specimens to determine the compressive,
as requirements of the standard. splitting tensile, and ﬂexural strength of in-place concrete.
1.4 This standard does not purport to address the safety 3.2 Generally, test specimens are obtained when doubt
concerns, if any, associated with its use. It is the responsibility exists about the in-place concrete quality due either to low
of the user of this standard to establish appropriate safety and strength test results during construction or signs of distress in
health practices and determine the applicability of regulatory the structure. Another use of this method is to provide strength
limitations prior to use. information on older structures.
3.3 Concrete strength is affected by the location of the
2. Referenced Documents concrete in a structural element, with the concrete at the bottom
2.1 ASTM Standards: tending to be stronger than the concrete at the top. Core
C 39/C 39M Test Method for Compressive Strength of Cy- strength is also affected by core orientation relative to the
lindrical Concrete Specimens2 horizontal plane of the concrete as placed, with strength
C 78 Test Method for Flexural Strength of Concrete (Using tending to be lower when measured parallel to the horizontal
Simple Beam with Third-Point Loading)2 plane.4 These factors shall be considered in planning the
C 174/C 174M Test Method for Measuring Length of locations for obtaining concrete samples and in comparing
Drilled Concrete Cores2 strength test results.
C 496 Test Method for Splitting Tensile Strength of Cylin- 3.4 The strength of concrete measured by tests of cores and
drical Concrete Specimens2 beams is affected by the amount and distribution of moisture in
C 617 Practice for Capping Cylindrical Concrete Speci- the specimen at the time of test. There is no standard procedure
mens2 to condition a specimen that will ensure that, at the time of test,
it will be in the identical moisture condition as concrete in the
1
This test method is under the jurisdiction of ASTM Committee C09 on
Concrete and Concrete Aggregates and is the direct responsibility of Subcommittee
3
C09.61 on Testing Concrete for Strength. Available from American Concrete Institute (ACI), P.O. Box 9094, Farmington
Current edition approved Jan. 10, 2003. Published April 2003. Originally Hills, MI 48333.
4
approved in 1921. Last previous edition approved in 1999 as C 42/C 42M-99. Neville, A., “Core Tests: Easy to Perform, Not Easy to Interpret,” Concrete
2
Annual Book of ASTM Standards, Vol 04.02. International, Vol. 23, No. 11, November 2001, pp. 59-68.
Copyright © ASTM International, 100 Barr Harbor Drive, PO Box C700, West Conshohocken, PA 19428-2959, United States.
1
C 42/C 42M – 03
structure. The moisture conditioning procedures in this test horizontal plane of the concrete as placed. A specimen drilled
method are intended to provide reproducible moisture condi- perpendicular to a vertical surface, or perpendicular to a
tions that minimize within-laboratory and between-laboratory surface with a batter, shall be taken from near the middle of a
variations and to reduce the effects of moisture introduced unit of deposit when possible.
during specimen preparation. 5.3 Slab Removal—Remove a slab sufficiently large to
3.5 There is no universal relationship between the compres- secure the desired test specimens without the inclusion of any
sive strength of a core and the corresponding compressive concrete that has been cracked, spalled, undercut, or otherwise
strength of standard-cured molded cylinders. The relationship damaged.
is affected by many factors such as the strength level of the
concrete, the in-place temperature and moisture history, and the DRILLED CORES
strength gain characteristics of the concrete. Historically, it has 6. Measuring the Length of Drilled Cores
been assumed that core strengths are generally 85 % of the
corresponding standard-cured cylinder strengths, but this is not 6.1 Cores for determining the thickness of pavements, slabs,
applicable to all situations. The acceptance criteria for core walls or other structural elements shall have a diameter of at
strength are to be established by the speciﬁer of the tests. ACI least 3.75 in. [95 mm] when the lengths of such cores are
318 provides core strength acceptance criteria for new con- stipulated to be measured in accordance with Test Method
struction. C 174/C 174M.
6.2 For cores that are not intended for determining structural
4. Apparatus dimensions, measure the longest and shortest lengths on the cut
surface along lines parallel to the core axis. Record the average
4.1 Core Drill, for obtaining cylindrical core specimens
length to the nearest 1⁄4 in. [5 mm].
with diamond impregnated bits attached to a core barrel.
4.2 Saw, for cutting beam specimens to size for ﬂexural 7. Cores for Compressive Strength
strength tests and to trim ends of cores. The saw shall have a
7.1 Diameter—The diameter of core specimens for the
diamond or silicon-carbide cutting edge and shall be capable of
determination of compressive strength in load bearing struc-
cutting specimens that conform to the prescribed dimensions,
tural members shall be at least 3.70 in. [94 mm]. For non-load
without excessive heating or shock.
bearing structural members or when it is impossible to obtain
cores with length-diameter ratio (L/D) greater than or equal to
5. Sampling
1, core diameters less than 3.70 in. [94 mm] are not prohibited
5.1 General: (see Note 3). For concrete with nominal maximum aggregate
5.1.1 Samples of hardened concrete for use in the prepara- size greater than or equal to 11⁄2 in. [37.5 mm], the core
tion of strength test specimens shall not be taken until the diameters shall be as directed by the speciﬁer of the tests (see
concrete is strong enough to permit sample removal without Note 4).
disturbing the bond between the mortar and the coarse aggre-
gate (see Note 1 and Note 2). When preparing strength test NOTE 3—The compressive strengths of nominal 2-in. [50-mm] diam-
eter cores are known to be somewhat lower and more variable than those
specimens from samples of hardened concrete, samples that
of nominal 4-in. [100-mm] diameter cores. In addition, smaller diameter
have been damaged during removal shall not be used unless the cores appear to be more sensitive to the effect of the length-diameter
damaged portion(s) are removed and the resulting test speci- ratio.5
men is of suitable length (see 7.2). Samples of defective or NOTE 4—The preferred minimum core diameter is three times the
damaged concrete that cannot be tested shall be reported along nominal maximum size of the coarse aggregate but it should be at least
with the reason that prohibits use of the sample for preparing two times the nominal maximum size of the coarse aggregate.
strength test specimens. 7.2 Length—The preferred length of the capped or ground
NOTE 1—Practice C 823 provides guidance on the development of a specimen is between 1.9 and 2.1 times the diameter. If the ratio
sampling plan for concrete in constructions. of the length to the diameter (L/D) of the core exceeds 2.1,
NOTE 2—It is not possible to specify a minimum age when concrete is reduce the length of the core so that the ratio of the capped or
strong enough to withstand damage during removal, because the strength ground specimen is between 1.9 and 2.1. Core specimens with
at any age depends on the curing history and strength grade of the length-diameter ratios equal to or less than 1.75 require
concrete. If time permits, the concrete should not be removed before it is corrections to the measured compressive strength (see 7.9.1). A
14 days old. If this is not practical, removal of concrete can proceed if the
cut surfaces do not display erosion of the mortar and the exposed coarse
strength correction factor is not required for L/D greater than
aggregate particles are embedded ﬁrmly in the mortar. In-place test 1.75. A core having a maximum length of less than 95 % of its
methods may be used to estimate the level of strength development prior diameter before capping or a length less than its diameter after
to attempting removal of concrete samples. capping or end grinding shall not be tested.
5.1.2 Specimens containing embedded reinforcement shall 7.3 Moisture Conditioning—Test cores after moisture con-
not be used for determining compressive, splitting tensile, or ditioning as speciﬁed in this test method or as directed by the
ﬂexural strength. speciﬁer of the tests. The moisture conditioning procedures
5.2 Core Drilling—A core specimen shall be drilled perpen-
dicular to the surface and not near formed joints or obvious 5
Bartlett, F.M. and MacGregor, J.G., “Effect of Core Diameter on Concrete Core
edges of a unit of deposit. Record and report the approximate Strengths,” ACI Materials Journal, Vol. 91, No. 5, September-October 1994, pp.
angle between the longitudinal axis of the drilled core and the 460-470.
2
C 42/C 42M – 03
speciﬁed in this test method are intended to preserve the core lengths to the nearest 0.1 in. [2 mm] before capping.
moisture of the drilled core and to provide a reproducible Unbonded caps in accordance with Practice C 1231/C 1231M
moisture condition that minimizes the effects of moisture are not permitted.
gradients introduced by wetting during drilling and specimen 7.7 Measurement—Before testing, measure the length of the
preparation. capped or ground specimen to the nearest 0.1 in. [2 mm] and
7.3.1 After cores have been drilled, wipe off surface drill use this length to compute the length-diameter (L/D) ratio.
water and allow remaining surface moisture to evaporate. Determine the average diameter by averaging two measure-
When surfaces appear dry, but not later than 1 h after drilling, ments taken at right angles to each other at the midheight of the
place cores in separate plastic bags or nonabsorbent containers specimen. Measure core diameters to the nearest 0.01 in. [0.2
and seal to prevent moisture loss. Maintain cores at ambient mm] when the difference in core diameters does not exceed
temperature, and protect cores from exposure to direct sunlight. 2 % of their average, otherwise measure to the nearest 0.1 in.
Transport the cores to the testing laboratory as soon as [2 mm]. Do not test cores if the difference between the largest
practicable. Keep cores in the sealed plastic bags or nonabsor- and smallest diameter exceeds 5 % of their average.
bent containers at all times except during end preparation and 7.8 Testing—Test the specimens in accordance with Test
for a maximum time of 2 h to permit capping before testing. Method C 39/C 39M. Test the specimens within 7 days after
coring, unless speciﬁed otherwise.
7.3.2 If water is used during sawing or grinding of core 7.9 Calculation—Calculate the compressive strength of
ends, complete these operations as soon as practicable, but no each specimen using the computed cross-sectional area based
later than 2 days after drilling of cores unless stipulated on the average diameter of the specimen.
otherwise by the speciﬁer of tests. After completing end 7.9.1 If the ratio of length to diameter (L/D) of the specimen
preparation, wipe off surface moisture, allow the surfaces to is 1.75 or less, correct the result obtained in 7.9 by multiplying
dry, and place the cores in sealed plastic bags or nonabsorbent by the appropriate correction factor shown in the following
containers. Minimize the duration of exposure to water during table (see Note 6):
end preparation. Ratio of Length Strength
7.3.3 Allow the cores to remain in the sealed plastic bags or to Diameter (L/D) Correction Factor
nonabsorbent containers for at least 5 days after last being 1.75 0.98
wetted and before testing, unless stipulated otherwise by the 1.50 0.96
speciﬁer of tests. 1.25 0.93
1.00 0.87
NOTE 5—The waiting period of at least 5 days is intended to reduce
Use interpolation to determine correction factors for L/D
moisture gradients introduced when the core is drilled or wetted during
sawing or grinding. values not given in the table.
NOTE 6—Correction factors depend on various conditions such as
7.3.4 When direction is given to test cores in a moisture
moisture condition, strength level, and elastic modulus. Average values for
condition other than achieved by conditioning according to corrections due to length-diameter ratio are given in the table. These
7.3.1, 7.3.2, and 7.3.3, report the alternative procedure. correction factors apply to low-density concrete having a density between
7.4 Sawing of Ends—The ends of core specimens to be 100 and 120 lb/ft3 [1600 and 1920 kg/m3] and to normal density concrete.
tested in compression shall be ﬂat, and perpendicular to the They are applicable to both dry and wet concrete for strengths between
2000 psi and 6000 psi [14 MPa to 42 MPa]. For strengths above 10000 psi
longitudinal axis. If necessary, saw the ends of cores that will
[70 MPa], test data on cores show that the correction factors may be larger
be capped so that the following requirements are met: than the values listed above.6
7.4.1 Projections, if any, shall not extend more than 0.2 in.
7.10 Report—Report the results as required by Test Method
[5 mm] above the end surfaces.
C 39/C 39M with the addition of the following information:
7.4.2 The end surfaces shall not depart from perpendicular- 7.10.1 Length of core as drilled to the nearest 1⁄4 in. [5 mm],
ity to the longitudinal axis by more than 0.5 degrees. 7.10.2 Length of test specimen before and after capping or
7.5 Density—When required by the speciﬁer of the tests, end grinding to the nearest 0.1 in. [2 mm], and average
determine the density by weighing the core before capping and diameter of core to the nearest 0.01 in. [0.2 mm] or 0.1 in. [2
dividing the mass by the volume of the core calculated from the mm],
average diameter and length. Alternatively, determine the 7.10.3 Compressive strength to the nearest 10 psi [0.1 MPa]
density from the mass in air and submerged mass in accordance when the diameter is measured to the nearest 0.01 in. [0.2 mm]
with Test Method C 642. After submerged weighing, dry cores and to the nearest 50 psi [0.5 MPa] when the diameter is
in accordance with 7.3.2 and store in sealed plastic bags or measured to the nearest 0.1 in. [2 mm], after correction for
nonabsorbent containers for at least 5 days before testing. length-diameter ratio when required,
7.6 Capping—If the ends of the cores do not conform to the 7.10.4 Direction of application of the load on the specimen
perpendicularity and planeness requirements of Test Method with respect to the horizontal plane of the concrete as placed,
C 39/C 39M, they shall be sawed or ground to meet those
requirements or capped in accordance with Practice C 617. If
cores are capped in accordance with Practice C 617, the 6
Bartlett, F.M. and MacGregor, J.G, “Effect of Core Length-to-Diameter Ratio
capping device shall accommodate actual core diameters and on Concrete Core Strengths,” ACI Materials Journal, Vol. 91, No. 4, July-August
produce caps that are concentric with the core ends. Measure 1994, pp. 339-348.
3
C 42/C 42M – 03
7.10.5 The moisture conditioning history:
7.10.5.1 The date and time core was obtained and ﬁrst
placed in sealed bag or nonabsorbent container,
7.10.5.2 If water was used during end preparation, the date
and time end preparation was completed and core placed in
sealed bag or nonabsorbent container,
7.10.6 The date and time when tested,
7.10.7 Nominal maximum size of concrete aggregate.
7.10.8 If determined, the density,
7.10.9 If applicable, description of defects in cores that
could not be tested, and
7.10.10 If any deviation from this test method was required,
describe the deviation and explain why it was necessary.
7.11 Precision:7
7.11.1 The single-operator coefficient of variation on cores
has been found to be 3.2 % 8 for a range of compressive
strength between 4500 psi [32.0 MPa] and 7000 psi [48.3
MPa]. Therefore, results of two properly conducted tests of
single cores by the same operator on the same sample of
material should not differ from each other by more than 9 % 8
of their average.
7.11.2 The multi-laboratory coefficient of variation on cores
has been found to be 4.7 % 8 for a range of compressive
strength between 4500 psi [32.0 MPa] and 7000 psi [48.3
MPa]. Therefore, results of two properly conducted tests on
cores sampled from the same hardened concrete (where a
single test is deﬁned as the average of two observations (cores),
each made on separate adjacent drilled 4 in. [100 mm] diameter
cores), and tested by two different laboratories should not differ
from each other by more than 13 % 8 of their average.
7.12 Bias—Since there is no accepted reference material
suitable for determining the bias for the procedure in this test
method, no statement on bias is being made.
8. Cores for Splitting Tensile Strength
8.1 Test Specimens—The specimens shall conform to the
dimensional requirements in 7.1, 7.2, 7.4.1 and 7.4.2. Ends are
not to be capped.
8.2 Moisture Conditioning—Condition the specimens as FIG. 1 Suitable Capping Device for Splitting Tensile Strength Test
described in 7.3, or as directed by the speciﬁer of tests.
8.3 Bearing Surfaces—The line of contact between the bearing surfaces of core specimens.
specimen and each bearing strip shall be straight and free of 8.4 Testing—Test the specimens in accordance with Test
any projections or depressions higher or deeper than 0.01 in. Method C 496.
[0.2 mm]. When the line of contact is not straight or contains 8.5 Calculation and Report—Calculate the splitting tensile
projections or depressions having heights or depths greater strength and report the results as required in Test Method
than 0.01 in., grind or cap the specimen so as to produce C 496. When grinding or capping of the bearing surfaces is
bearing lines meeting these requirements. Do not test speci- required, measure the diameter between the ﬁnished surfaces.
mens with projections or depressions greater than 0.1 in. [2.0 Indicate that the specimen was a core and provide the moisture
mm]. When capping is employed, the caps shall be as thin as conditioning history as in 7.10.5.
practicable and shall be formed of high-strength gypsum 8.6 Precision:9
plaster. 8.6.1 The within laboratory single operator coefficient of
NOTE 7—Fig. 1 illustrates a device suitable for applying caps to the variation for splitting tensile strength between 520 psi [3.6
MPa] and 590 psi [4.1 MPa] of cores has been found to be
5.3 %.8 Therefore, results of two properly conducted tests by
7
Bollin, G. E., “Development of Precision and Bias Statements for Testing
Drilled Cores in Accordance with ASTM C 42,” ASTM Journal of Cement,
9
Concrete, and Aggregates, Vol 15, No. 1, 1993. Steele, G.W., “Portland Cement Concrete Core Proﬁciency Sample Program,”
8
These numbers represent, respectively, the (1s %) and (d2s %) limits as Strategic Highway Research Program, SHRP-P-636, National Research Council,
described in Practice C 670. Washington, D.C., 1993.
4
C 42/C 42M – 03
the same operator in the same laboratory on the same sample the period between removal from water storage and testing,
of material should not differ by more than 14.9 % 8 of their keep the specimens moist by covering with a wet blanket of
average. burlap or other suitable absorbent fabric.
8.6.2 The multi-laboratory coefficient of variation for split- 9.2.1 When the speciﬁer of tests so directs, beams shall be
ting tensile strength between 520 psi [3.6 MPa] and 590 psi tested in a moisture condition other than that achieved by
[4.1 MPa] of cores has been found to be 15.0 %.8 Therefore, conditioning in accordance with 9.2.
results of two properly conducted tests on the same sample of NOTE 9—Relatively small amounts of drying of the surface of ﬂexural
material of hardened concrete and tested by two different specimens induce tensile stresses in the extreme ﬁbers that will markedly
laboratories should not differ from each other by more than reduce the indicated ﬂexural strength.
42.3 % 8 of their average.
9.3 Testing—Test the specimens in accordance with the
8.7 Bias—Since there is no accepted reference material
applicable provisions of Test Method C 78.
suitable for determining the bias for the procedure in this test
method, no statement on bias is being made. NOTE 10—Sawing may greatly reduce the indicated ﬂexural strength;
beams shall, therefore, be tested with a molded surface in tension
BEAMS FOR FLEXURAL TESTING whenever possible. The location of the tension face with respect to the
position of the concrete as placed and the position of the sawed surfaces
should be reported.
9. Flexural Strength
9.4 Report—Report the results in accordance with the
9.1 Test Specimens—Unless otherwise speciﬁed, a beam
applicable provisions of Test Method C 78 and the require-
specimen for the determination of ﬂexural strength shall have
ments of this test method, including the moisture condition at
a nominal cross section of 6 by 6 in. [150 by 150 mm] (Note
the time of testing. Identify orientation of the specimen’s
8). The specimen shall be at least 21 in. [530 mm] in length, but
ﬁnished, sawed, and tension faces with respect to their posi-
when two tests for ﬂexural strength are to be made in one beam
tions in the test apparatus.
specimen, it shall be at least 33 in. [840 mm] in length. Perform
the sawing operation so that the concrete will not be weakened 10. Precision and Bias
by shock or by heating. The sawed surfaces shall be smooth, 10.1 Precision—Data are not available for preparing a
plane, parallel, and free from steps, ridges, and grooves. Take statement on the precision of ﬂexural strength measured on
care in handling sawed beam specimens to avoid chipping or sawed beams.
cracking.
NOTE 11—Users of this method who have replicate test data that may
NOTE 8—In many cases, particularly with prisms cut from pavement be appropriate for a statement on repeatability are encouraged to contact
slabs, the width will be governed by the size of the coarse aggregate and the chairman of the subcommittee.
the depth by the thickness of the slab.
10.2 Bias—Since there is no accepted reference material
9.2 Moisture Conditioning—Protect the surfaces of sawed suitable for determining the bias for the procedure in this test
specimens from evaporation by covering them with wet burlap method, no statement on bias is being made.
and plastic sheeting during transportation and storage. Test the
specimens within 7 days of sawing. Submerge the test speci- 11. Keywords
mens in lime-saturated water at 73.5 6 3.5°F [23.06 2.0°C] 11.1 compressive strength; concrete coring; concrete saw-
for at least 40 h immediately prior to the ﬂexure test. Test the ing; concrete strength; ﬂexural strength; splitting tensile
specimens promptly after removal from water storage. During strength
ASTM International takes no position respecting the validity of any patent rights asserted in connection with any item mentioned
in this standard. Users of this standard are expressly advised that determination of the validity of any such patent rights, and the risk
of infringement of such rights, are entirely their own responsibility.
This standard is subject to revision at any time by the responsible technical committee and must be reviewed every ﬁve years and
if not revised, either reapproved or withdrawn. Your comments are invited either for revision of this standard or for additional standards
and should be addressed to ASTM International Headquarters. Your comments will receive careful consideration at a meeting of the
responsible technical committee, which you may attend. If you feel that your comments have not received a fair hearing you should
make your views known to the ASTM Committee on Standards, at the address shown below.
This standard is copyrighted by ASTM International, 100 Barr Harbor Drive, PO Box C700, West Conshohocken, PA 19428-2959,
United States. Individual reprints (single or multiple copies) of this standard may be obtained by contacting ASTM at the above
address or at 610-832-9585 (phone), 610-832-9555 (fax), or service@astm.org (e-mail); or through the ASTM website
(www.astm.org).
5
![](images/graphics/blank.gif)
![](images/graphics/blank.gif)
[Tuyển tập các tiêu chuẩn về đất xây dựng công trình thủy lợi - Từ 14 TCN 123-2002 đến 14 TCN 129-2002](http://tailieu.vn/bst/tuyen-tap-cac-tieu-chuan-ve-dat-xay-dung-cong-trinh-thuy-loi-tu-14-tcn-123-2002-den-14-tcn-129-200-250439.html)
## Top Download Tiêu Chuẩn - Qui Chuẩn
-
-
39p
4123
803
-
[TIÊU CHUẨN ĐÁNH GIÁ HIỆU QUẢ DỰ ÁN ĐẦU TƯ](http://tailieu.vn/doc/tieu-chuan-danh-gia-hieu-qua-du-an-dau-tu-470097.html)
7p
771
252
-
[Các tiêu chuẩn quản lý môi trường ISO 14000](http://tailieu.vn/doc/cac-tieu-chuan-quan-ly-moi-truong-iso-14000-67088.html)
29p
2088
1072
-
-
[Hệ thống quản lý chất lượng theo ISO 9000](http://tailieu.vn/doc/he-thong-quan-ly-chat-luong-theo-iso-9000-67092.html)
3p
2539
720
-
-
-
-
Tài Liệu Tiêu chuẩn - Qui Chuẩn Mới
[Xem thêm »](http://tailieu.vn/kinh-te-quan-ly/tieu-chuan-qui-chuan/)
Tài Liệu mới cập nhật
[Xem thêm »](http://tailieu.vn/tai-lieu/)
-
-
-
-
[Tiêu chuẩn Kỹ thuật điện nông thôn](http://tailieu.vn/doc/tieu-chuan-ky-thuat-dien-nong-thon-1637115.html)
110p
2
1
-
-


markdown:
Công ty cổ phần tập đoàn vật liệu chịu lửa Thái Nguyên
Công ty cổ phần tập đoàn Vật liệu chịu lửa Thái nguyên là nhà sản xuất hàng đầu Việt Nam về các sản phẩm vật liệu chịu lửa( gạch chịu lửa, bê tông chịu lửa, vữa chịu lửa, sạn chịu lửa ).
Sản phẩm vật liệu chịu lửa của Công ty được cung cấp rộng rãi cho thị trường trong cả nước, phục vụ cho nhiều lĩnh vực, trong đó có các ngành như : luyện kim, xi măng, hóa chất, vật liệu xây dựng, gốm sứ, và các ngành công nghiệp khác....
Bên cạnh đó Công ty còn sản xuất các mặt hàng vật liệu chịu lửa - gạch chịu lửa cao cấp phục vụ cho các đơn vị liên doanh của nước ngoài tại Việt Nam và xuất khẩu sang các nước như : Hàn quốc , Đài loan, Nhật Bản, Indonexia ...
Công ty có dây chuyền thiết bị hiện đại khép kín từ khâu gia công nguyên liệu, tạo hình và nung sản phẩm. Với hệ thống máy ép thủy lực 630 tấn, 1600 tấn và máy ép ma sát 500 tấn,630 tấn, 1200 tấn và 2000 tấn của Mỹ, Nga, Đức và Trung Quốc sản xuất .
Hệ thống lò nung con thoi, lò nung Tuynel hiện đại điều khiển bằng PLC và máy tính công nghiệp ( nhiệt độ của lò nung con thoi max 1800 độ, nhiệt độ lò nung Tuynel max 1650 độ ).
Mỗi năm Công ty sản xuất và tiêu thụ 60.000 tấn - 65.000 tấn vật liệu chịu lửa các loại. Công ty thường xuyên đổi mới công nghệ, đầu tư thiết bị hiện đại để nâng cao chất lượng sản phẩm, đáp ứng tốt nhất nhu cầu ngày càng khắt khe của thị trường .
Các mặt hàng sản phẩm của Công ty đang sản xuất và tiêu thụ gồm :
+ Gạch chịu lửa có hàm lượng cao nhôm 50-85 %.
+ Gạch chịu lửa Sa mốt A, B.
+ Gạch MgO-C
+ Gạch MgO- Cr2O3.
+ Gạch MgO Spinel
+ Gạch xốp nhẹ.
+ Gạch chịu axit.
+ Gạch Đinát
+ Tấm cách nhiệt Canxiumxilicats
+ Các sản phẩm bê tông chịu lửa
+ Bột,vữa,sạn chịu lửa các loại.
...
Ngoài ra, Công ty còn sản xuất vôi, Đôlômít luyện kim dùng cho ngành luyện kim. Công ty có đội ngũ cán bộ kỹ sư giàu kinh nghiệm thuộc nhiều ngành nghề được đào tạo qua các trường đại học trong và ngoài nước .
Công ty nhận thiết kế xây dựng và lắp đặt sửa chữa các lò công nghiệp và thiết bị nhiệt .

WARC-Type: response

Content-Type: application/http; msgtype=response

Connection: close

Cache-Control: private

Content-Type: text/html; charset=utf-8


markdown:
|
|
|
|
«
»
|Thread
||Thread Starter
||Forum
||Replies
||Last Post
||greenlife
||Kiểm tra chất lượng,giám định hàng hóa,sở hữu trí tuê
||4
||09-26-2012 14:24
||huytrn11
||Hàng phi mậu dịch
||3
||07-14-2011 16:17
||sonnq74
||Xây dựng diễn đàn
||0
||03-21-2011 08:44
||yushironaka
||Hàng thương mại
||4
||01-18-2011 00:30
||maihung
||Hàng thương mại
||2
||08-09-2010 14:28
|
All times are GMT +7. The time now is 22:31.

Content-Type: text/html; charset=ISO-8859-1

Set-Cookie: bblastactivity=0; expires=Fri, 17-Apr-2015 15:31:02 GMT; path=/

Pragma: private

Content-Encoding: gzip


markdown:
10:53 | Thứ ba 16/01/2007 (GMT+7)
Trong suốt nhiều thế kỷ qua,
**Anh và Pháp** luôn ganh đua với nhau về lãnh thổ và quyền lực. Tuy nhiên, theo một tài liệu mật mới được tiết lộ, hai đối thủ lâu năm từng có ý hợp nhất thành một nước vào những năm 1950.
07:11 | Thứ sáu 09/03/2007 (GMT+7)
Đúng như dự đoán, ĐKVĐ Sevilla đã tỏ rõ sự không mặn mà với giải cúp "hạng hai" của Châu Âu và chỉ hòa 2-2 với đối thủ Shakhtar Donetsk. Các đại diện khác của La Liga như Espanyol, Celta Vigo và Osasuna cũng chỉ từ hòa tới thua. Trong khi đó, các đại diện của bóng đá
**Anh và Pháp** đều giành được những kết quả có lợi, qua đó có ưu thế rất lớn để ghi tên mình vào vòng tứ kết cúp UEFA.
10:32 | Thứ ba 24/02/2004 (GMT+7)
Orange, công ty viễn thông lớn thứ 3 châu Âu, tuyên bố đã bắt đầu triển khai mạng điện thoại thế hệ 3 (3G) phủ sóng hơn 20 thành phố lớn ở
**Anh và Pháp**. Song song với động thái này, Orange cũng đã lên kế hoạch tung ra thị trường hàng loạt điện thoại di động 3G trong 6 tháng cuối năm nay.
06:32 | Thứ năm 09/09/2004 (GMT+7)
Sau trận hoà đáng thất vọng cuối tuần trước,
**Anh và Pháp** đều kiếm được chiến thắng đầu tiên ở vòng loại World Cup đêm qua, lần lượt trên sân của Ba Lan và đảo Faroe, với tỷ số 2-1 và 2-0. Giành ba điểm, các cầu thủ cũng như HLV hai đội phần nào giảm được áp lực từ phía người hâm mộ.
08:19 | Thứ năm 08/02/2007 (GMT+7)
Trong khi Đức đánh bại chủ nhà EURO 2008 Thụy Sĩ 3-1 thuyết phục thì
**Anh và Pháp** lại để thua trước 2 đối thủ cứng cựa là Tây Ban Nha và Argentina trên sân nhà.
22:30 | Thứ tư 17/01/2007 (GMT+7)
Thông tin về việc Pháp từng có ý định hợp nhất với Anh cách đây nửa thế kỷ để trở thành một quốc gia đã khiến giới sử gia sửng sốt. Trong nhiều thế kỷ qua, hai nước này luôn tranh cãi về lãnh thổ và nhiều vấn đề khác, vậy lý do gì khiến "gà trống Gaulois" muốn "kết hôn" cùng nước láng giềng?
07:20 | Thứ bảy 12/05/2007 (GMT+7)
Vào lúc 16h chiều ngày 15/5, Đại sứ quán
**Anh và Pháp** cùng đoàn tuỳ tùng sẽ có chuyến công tác đến TP.Pleiku để thăm học viện bóng đá HA.GL-Arsenal JMG. Sở dĩ CLB HA.GL vinh dự được chọn là đích đến trong chuyến viếng thăm này, là vì trong thời gian qua, trên một số phương tiện thông tin đại chúng của cả **Anh và Pháp**, như BBC, Paris Match… liên tục có những tin bài khen ngợi về một doanh nghiệp thành đạt làm bóng đá như HA.GL Group của bầu Đức.
10:32 | Thứ bảy 08/10/2005 (GMT+7)
Tổng Thống Pháp Jacques Chirac và Thủ Tướng Anh Tony Blair cam kết gạt những điểm bất đồng sang một bên và cùng nhau làm việc cho lợi ích của Liên Hiệp Âu Châu.
01:36 | Chủ nhật 03/09/2006 (GMT+7)
Quá dễ cho McClaren và các học trò trong trận ra quân ở một giải đấu chính thức khi đối thủ đầu tiên của họ ở vòng loại EURO 2008 chỉ là chú bé hạt tiêu Andorra.
01:16 | Thứ tư 16/05/2007 (GMT+7)
Trong chuyến đi công tác tại các tỉnh Tây nguyên để thúc đẩy việc hợp tác đầu tư và phát triển kinh tế, Đại sứ đặc mệnh toàn quyền Vương quốc Anh - ngài Robert Gordon, và Đại sứ đặc mệnh toàn quyền Cộng hòa Pháp - ngài Jean - Franøois Blarel, đã đến thăm và tìm hiểu về tiềm lực của CLB Hoàng Anh Gia Lai vào chiều 15-5.
07:22 | Thứ ba 16/01/2007 (GMT+7)
Các tài liệu mới được tìm thấy cho biết
**Anh và Pháp** từng tính đến khả năng hợp lại thành một khối vào thập kỷ 1950.
09:18 | Thứ tư 01/06/2005 (GMT+7)
Cú hat-trick của Michael Owen giúp tuyển Anh đánh bại Colombia 3-2. Như vậy, đội tuyển xứ sở sương mù đã kết thúc chuyến du đấu rất thành công trên đất Mỹ, với hai chiến thắng cùng màn ra mắt ấn tượng của các tài năng trẻ. Pháp có chiến thắng đầu tiên trên sân nhà dưới triều đại của HLV Domenech.
00:07 | Thứ tư 07/09/2005 (GMT+7)
"Những chú gà trống" Gaulois đến Cộng hòa Ireland để quyết đấu trong khi Anh phải bước qua xác Bắc Ireland và còn hy vọng tranh ngôi đầu bảng.
07:46 | Thứ tư 01/06/2005 (GMT+7)
Cú hat-trick của Michael Owen giúp tuyển Anh đánh bại Colombia 3-2. Như vậy, đội tuyển xứ sở sương mù đã kết thúc chuyến du đấu rất thành công trên đất Mỹ, với hai chiến thắng cùng màn ra mắt ấn tượng của các tài năng trẻ. Pháp có chiến thắng đầu tiên trên sân nhà dưới triều đại của HLV Domenech.
23:11 | Thứ sáu 01/12/2006 (GMT+7)
Phóng viên TTXVN tại Vương quốc Anh cho biết lệnh cấm hút thuốc lá tại các địa điểm công cộng trên toàn nước Anh sẽ bắt đầu có hiệu lực từ ngày 1/7/2007.
18:45 | Thứ tư 16/05/2007 (GMT+7)
TP - Chiều qua (15/5) nhân chuyến công tác 3 tỉnh Tây Nguyên: Đắc Lắc, Gia Lai, Kontum, hai Đại sứ đặc mệnh toàn quyền Vương quốc Anh Robert Gordon và Cộng hoà Pháp Jean Francois Blarel đã chủ động đề nghị thăm CLB Hoàng Anh Gia Lai (HAGL).
09:30 | Chủ nhật 05/09/2004 (GMT+7)
Hai đại gia này đều có sự khởi đầu đáng thất vọng tại vòng loại World Cup 2006 khu vực châu Âu, đêm qua. Pháp bị Israel cầm chân ngay trên sân nhà, với tỷ số 0-0. Còn đội bóng của quốc đảo sương mù phải chấp nhận kết quả 2-2, sau khi đã dẫn trước hai bàn.
16:20 | Thứ năm 11/05/2006 (GMT+7)
Theo nguồn tin của báo Lao Động, hiện nay cả Thủ tướng Anh Tony Blair và Thủ tướng Pháp Dominique de Villepin đều đang đối mặt với những áp lực từ chức nặng nề nhất trong sự nghiệp chính trị của mình.
16:06 | Chủ nhật 13/06/2004 (GMT+7)
Trận cầu được mọi người mong đợi nhất ở vòng 1 này là trận Anh - Pháp ở bảng B, sẽ diễn ra vào lúc 1h45 ngày 14/6. Đây là trận cầu rất được nhiều người hâm mộ bóng đá mong đợi (theo một số người thì đây là trận đấu hay nhất vòng 1). Đây là lần thứ hai hai đội tuyển
**Anh và Pháp** gặp nhau từ trước đến nay tại Euro. Vậy hai ông khổng lồ đã chuẩn bị những gì cho trận gặp này?
08:40 | Thứ sáu 15/07/2005 (GMT+7)
Hôm qua, 14-7, Yahoo đã ra mắt phiên bản thử nghiệm beta phần mềm phiên dịch ngôn ngữ tiếng Đức sang tiếng
**Anh và Pháp**, và cho kết quả trên toàn thế giới bằng tiếng Đức.
Nạn nhân vụ Cát Tường bị rạch bụng sau khi chết?; Hoãn phiên xử bầu Kiên và đồng phạm; Ông Trần Xuân Giá khai gì về bầu Kiên?; Nổ súng xối xả trong nhà nghỉ chấn động Cần Thơ; Tai nạn thảm khốc trên cao tốc, 5 người chết...
Ông Võ Văn Thưởng nhậm chức Phó bí thư TP.HCM; Hợp long cầu dây văng lớn nhất Việt Nam; Hoang mang số liệu trẻ tử vong do dịch sởi; Hà Nội: Cháy lớn tại khu công nghiệp Vĩnh Tuy
Bộ Giáo dục xin 34 nghìn tỷ đổi mới chương trình; Dừng xử vụ Cát Tường, trả hồ sơ điều tra bổ sung; Chết tức tưởi sau khi bác sĩ rút 3 lọ tủy sống; Hai ca sỹ bị cướp giữa Sài Gòn...
Đường Trường Chinh bị nắn cong như thế nào; Nóng trước phiên xử vụ Cát Tường; Kỳ lạ hai xe ô tô chung biển số xanh “san bằng tất cả”; Nữ sinh mang thai ngất ở lớp rồi tử vong; Vì sao không công bố dịch sởi?...
Thanh tra lên tiếng vụ đường cong Trường Chinh; Hơn 100 chiến sỹ giải cứu 4 công an bị dân vây đánh; Hé lộ cát-sê khủng mời Khánh Ly về nước biểu diễn; Hy hữu: Bị hiếp dâm, bé gái quay clip tố cáo 'yêu râu xanh'
Theo kênh thông tin riêng của PV, Phòng PC45 (Công an tỉnh Ninh Bình) phát hiện tại CLB bóng đá Xi măng The Vissai Ninh Bình (thuộc Công ty TNHH Hoàng Phát Thể Thao) trong quá trình thi đấu bóng đá ở các giải V.league
Người dùng của một số website, dịch vụ trực tuyến lớn được khuyến khích đổi mật khẩu nhằm tự bảo vệ trước lỗ hổng Heartbleed.
Thời gian qua, thương lái Trung Quốc đến các vùng quê Việt Nam thu mua nhiều mặt hàng nông sản một cách không bình thường.
Chỉ vì mẫu thuẫn gia đình, nhát dao oan nghiệt đã cướp đi sinh mạng người con trai, đẩy cha già ở tuổi gần đất xa trời rơi vào vòng lao lý.
Gia đình Hà là một gia đình danh giá, chủ một hãng taxi lớn, một tiệm vàng trên đường Trường Chinh và một quán net tại số 270 Thiên Lôi.
Diễn biến dịch sởi: Lớn nhất mấy chục năm qua; Thiếu thuốc đặc trị ngộ độc nấm, nhiều bệnh nhân chết oan?; Vì sao không nên nấu nướng bằng nồi nhôm?; Giữ dáng người bằng ánh nắng mặt trời; Cận cảnh: Từ đuôi bò thối thành đặc sản!; 6 biểu hiện của "cậu nhỏ" không khỏe mạnh; 11 loại nước uống chống bức xạ máy tính... là những tin sức khỏe nổi bật tuần qua.
Đau lòng những vụ án cha mẹ giết con; Những thảm án cuồng yêu ở Sài Gòn; “Áp lực” tại phiên xử 5 công an đánh chết người đến từ đâu?; Ép cung, nhục hình: Căn nguyên của án oan!; 9X giết bạn, phi tang xác trong bể nước; Vụ TMV Cát Tường là án chưa từng có trong lịch sử tố tụng Việt Nam;...........là những tin đáng chú ý trong tuần.
Chỉ vì ham chơi và không làm bài tập về nhà, cậu bé 6 tuổi đã bị mẹ dùng móc treo quần áo đánh đập một cách dã man.
Cùng với việc kỳ công để theo đuổi, mời mọc ca sĩ Khánh Ly về nước biểu diễn, mức cát-sê của danh ca này cũng được hiểu là không hề nhỏ, nếu như không muốn nói là cao nhất từ trước đến nay dành cho các ca sĩ hải ngoại.
15 ngân hàng Việt Nam bị hacker tấn công, sau sự việc dưa hấu được mùa mất giá, đến lượt cà chua Đà Lạt đổ cho bò ăn, giá xăng giữ nguyên trong khi giá dầu giảm nhẹ, ngân hàng nóng chuyện mua bán - sáp nhập và tái cơ cấu... là những tin tức - sự kiện kinh tế nóng hổi trong tuần vừa qua.

WARC-Truncated: length